Rich Structural Chemistry in New Alkali Metal Yttrium Tellurites: Three-Dimensional Frameworks of NaYTe4O10, KY(TeO3)2, RbY(TeO3)2, and a Novel Variant of Hexagonal Tungsten Bronze, CsYTe3O8.
Kim, Youngkwon; Lee, Dong Woo; Ok, Kang Min; Inorganic chemistry 54 (2015) 389–395; doi:10.1021/ic502724n

data_4341955
_publ_section_title
;
 Rich Structural Chemistry in New Alkali Metal Yttrium Tellurites:
 Three-Dimensional Frameworks of NaYTe4O10, KY(TeO3)2, RbY(TeO3)2, and a
 Novel Variant of Hexagonal Tungsten Bronze, CsYTe3O8.
;
_journal_issue                   1
_journal_name_full               'Inorganic chemistry'
_journal_page_first              389
_journal_page_last               395
_journal_paper_doi               10.1021/ic502724n
_journal_volume                  54
_journal_year                    2015
_chemical_formula_sum            'O6 Rb Te2 Y'
_chemical_formula_weight         525.58
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.7281(3)
_cell_length_b                   6.0414(2)
_cell_length_c                   8.6320(2)
_cell_measurement_temperature    298(2)
_cell_volume                     715.91(3)
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 1
_diffrn_measurement_device_type  'Bruker SMART Breeze'
_diffrn_measurement_method       CCD
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0642
_diffrn_reflns_Laue_measured_fraction_full 1
_diffrn_reflns_Laue_measured_fraction_max 1
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            12714
_diffrn_reflns_point_group_measured_fraction_full 1
_diffrn_reflns_point_group_measured_fraction_max 1
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.328
_diffrn_reflns_theta_min         2.787
_exptl_absorpt_coefficient_mu    22.860
_exptl_absorpt_correction_T_max  0.60
_exptl_absorpt_correction_T_min  0.44
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details
; 
 SADABS(Blessing, 1995) 
;
_exptl_crystal_colour            Colorless
_exptl_crystal_density_diffrn    4.876
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Rod
_exptl_crystal_F_000             912
_exptl_crystal_size_max          0.034
_exptl_crystal_size_mid          0.031
_exptl_crystal_size_min          0.021
_refine_diff_density_max         0.594
_refine_diff_density_min         -0.741
_refine_diff_density_rms         0.164
_refine_ls_extinction_coef       0.00072(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.013
_refine_ls_matrix_type           full
_refine_ls_number_parameters     56
_refine_ls_number_reflns         973
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.013
_refine_ls_R_factor_all          0.0233
_refine_ls_R_factor_gt           0.0184
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0187P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0401
_refine_ls_wR_factor_ref         0.041
_reflns_number_gt                838
_reflns_number_total             973
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ic502724n_si_002.cif
_cod_data_source_block           RbYTe2O6
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'EMPIRICAL' changed to
'empirical' according to
/home/saulius/struct/COD-crude-data--automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2935 2014-11-11 08:27:57Z andrius 

 Adding full bibliography for 4341953--4341956.cif.
;
_cod_database_code               4341955